advertisement

International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 02 | Feb 2019 p-ISSN: 2395-0072 www.irjet.net Concrete Mix Design for M35 Grade: Comparison of Indian Standard Codes, IS 10262: 2009 & IS 456:2000 with American Code, ACI 211.1-91 Dada S. Patil Assistant Professor, Civil Engineering Department, Anjuman-I-Islam’s Kalsekar Technical Campus, School of Engineering & Technology, Panvel, Navi Mumbai, Maharashtra, India ---------------------------------------------------------------------***---------------------------------------------------------------------2. MIX DESIGN BY USING IS 10262: 2009 & IS Abstract - A rational & logical Concrete Mix Design to 456:2000 cater to the practical requirements plays a key role in concrete engineering. It is well established fact that the concrete is highly consumed material throughout the world. With the exponentially high demand of infrastructure facilities, the concrete requirement is on a very huge scale. Therefore, using the optimum quantities of concrete making constituent materials is of utmost importance in order to achieve the desired fresh & hardened properties. Owing to an enormous utilization of concrete in day- to-day construction work, economy is a vital factor to be considered. In India, mix design is carried out by following the rules prescribed in IS 10262: 2009 & IS 456:2000. As a well known fact, every country has its own codes to design a concrete mix. In this paper, an attempt has been made to compare the Concrete Mix Design of M35 grade by the American Code; ACI 211.1-91 with Indian codes IS 10262: 2009 & IS 456:2000. The outcomes are critically reviewed & the comments are given. 2.1 Stipulations for Proportioning Grade designation: M 35 Type of cement: Ordinary Portland Cement (OPC), conforming to IS: 12269-1987 Maximum nominal size of aggregate: Exposure condition considered: Moderate (for Reinforced Concrete) For moderate exposure condition (from Table 5 of IS 456: 2000) i) Minimum cement content: ii) Maximum water-cement ratio: 0.50. Desired workability: Type of aggregate: Crushed angular aggregate Keywords: OPC, (w/c) ratio, nominal maximum size of aggregate, workability, slump, target mean strength, etc. Maximum cement content: 450 kg/m3 (Clause 8.2.4.2 of IS 456: 2000) 1. INTRODUCTION 2.2 Test Data for Materials Every country has a peculiar method of carrying out the Concrete Mix Design by following the various clauses, tables & figures given in the codes of that particular country. It is obvious that these codes give important guidelines for designing a concrete mix depending upon the basic properties of constituent materials, behaviour of individual constituent, economy & many other considerations. The guidelines are proposed in such a way that the concrete is workable enough for a particular type of field application when it is in a fresh state; moreover, it caters to the need of desirable strength & durability properties, when hardened. This paper critically compares the Concrete Mix Design of M35 grade carried out by using Indian Standard codes & American code. The vital observations are presented. Conclusions are drawn based on these observations. © 2019, IRJET | Impact Factor value: 7.211 Specific gravity of cement: 3.15 Chemical admixture: NA Specific gravity of i) Coarse aggregate: 2.72 ii) Fine aggregate: 2.68 Sieve Analysis (coarse aggregates; 20 mm & 10 mm): Conforming to grading requirements of table 4 of IS 383:1970. Sieve analysis (Fine aggregates): Conforming to grading Zone I of table 4 of IS 383: 1970. | ISO 9001:2008 Certified Journal | Page 2580 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 02 | Feb 2019 p-ISSN: 2395-0072 www.irjet.net 2.3 Target Strength for Mix Proportioning 2.6 Proportion of Volume of Coarse Aggregate & Fine Aggregate Content fck’ = fck + (1.65 S) Where: From Table 3 of IS 10262: 2009, the volume of coarse = Target average compressive strength at 28 days. aggregates corresponding to = Characteristic compressive strength at 28 days aggregates of Zone I for (w/c) ratio of 0.50 is 0.60 . = Standard deviation. (w/c) ratio adopted is 0.45. Therefore, Volume of coarse From Table 1 of IS 102602: 2009, Standard deviation = ⁄ aggregate is required to be increased to decrease the fine , For M35 concrete aggregate content. As the water-cement ratio is lower by Therefore, target strength = = size aggregates & fine 0.05, the proportion of volume of coarse aggregate is to be ⁄ increased by 0.01 (at the rate of -/+ 0.01 for every ± 0.05 2.4 Selection of Water - Cement Ratio & Water change in water-cement ratio). Content Therefore, corrected proportion of volume of coarse From Table 5 of IS 456:2000, maximum water-cement aggregate for the water-cement ratio of 0.45 = (0.60 + ratio = 0.50 0.01) = 0.61. Adopt water-cement ratio as 0.45, since the target strength is 43.25 Volume of fine aggregate content = 1 - 0.61 = 0.39 N/mm2. 2.7 Mix Calculations From Table 2 of IS10262:2009, maximum water content = The mix calculations per unit volume of concrete shall be for as follows: aggregates. Volume of concrete (a) As per clause 4.2 of IS 10262:2009, for every increase of of cement) X (1/1000) 3%. ( . Volume of cement (b) = (mass of cement/ specific gravity slump of 25 mm, the water content has to be increased by So, estimated water content for = = (426.67 / 3.15) X (1/1000) = 0.135 m3. slump = Volume of water (c) = (mass of water/ specific gravity of ) water) X (1/1000) = = (192/1) X (1/1000) = 0.192 m3. Consider it as 192 kg/m3 Volume of all in aggregate (d) 2. 5 Calculation of Cement = 1 – (0.135 + 0.192) = 0.673 m3. Water-cement ratio = 0.45; Mass of coarse aggregate = (d) X volume of CA X specific Cement content = (192/0.45) = 426.67 kg/m3. gravity of CA X 1000. 450 kg/m3 (max. OPC permitted) > 426.67 kg/m3 > 300 = (0.673 X 0.61 X 2.72 X 1000) = 1116.64 kg. kg/m3 (min. cement content). Its complying the Mass of fine aggregate requirements. gravity of FA X 1000. = a – (b +c) = (d) X volume of FA X specific = (0.673 X 0.39 X 2.68 X 1000) = 703.42 kg. Yield of concrete = (426.67 + 192 + 703.42 + 1116.64) = 2438.73 kg/m3. © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 2581 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 02 | Feb 2019 p-ISSN: 2395-0072 www.irjet.net 2.8 Mix Proportions (kg/m3), at SSD (Saturated Table 3: Approximate Mixing Water & Air Content Surface Dry) condition of Fine Aggregate & Requirements for Different Slumps & Nominal Max. Size of Aggregates (SI Units) Coarse Aggregate Table 1: Mix Proportions Cement Water FA CA (w/c) ratio 426.67 192 703.42 1116.64 0.45 1 0.45 1.648 2.617 0.45 3. MIX DESIGN BY USING ACI 211.1-91 3.4 Selection of Water-Cement Ratio Let us carry out Mix Design by using ACI code. Let all the material properties be same as that in IS code method. Let dry rodded density of CA be 1640 kg/m3. Table 4: Relationship Between (w/c) Ratio & Compressive Strength of Concrete (SI Units) American code uses the concept of dry rodded density of CA. 3.1 Choice of Slump Table 2: Recommended Slumps for various Types of Construction (SI Units) For target strength of 43.25 N/mm2, (w/c) ratio for nonair entrained concrete is 0.54, by interpolation. This is more than the maximum (w/c) ratio of 0.50 for the moderate exposure condition, as given by the Indian Code. If the (w/c) ratio given by ACI method exceeds the maximum limit of 0.50 prescribed by the Indian Standard Code (moderate exposure), the value should be discarded & (w/c) ratio of 0.50 is to be used for further calculations. Though ACI method is used for the Mix Design, the Desired slump is 75 mm (25 mm to 75 mm category from concreting is to be done in India & therefore, the exposure table 2). conditions must be considered from the Indian Code from 3.2 Choice of Maximum Size of Aggregate durability point of view. However, if the (w/c) ratio From table 3, select Max. Aggregate Size = 19 mm, as it is obtained by ACI method is less than the max. limit given by closer to 20 mm size. IS code table, it is obvious that the value obtained is to be 3.3 Estimation of Mixing Water & Air Content adopted for further calculations. From table 3, W=205 litres (i. e. kg) for 19 mm aggregates 3.5 Calculation of Cement Content & entrapped air = 2%. Mass of cement, MC = Water/ {w/c ratio} = (205/0.50) = 410 kg/m3. © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 2582 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 02 | Feb 2019 p-ISSN: 2395-0072 www.irjet.net Here, the (w/c) ratio is marginally more than that in IS 3.7 Mix Proportions (kg/m3), at SSD (Saturated method. It is well established fact that, as the (w/c) ratio Surface Dry) condition of Fine Aggregate & increases, the strength shows decline in its value. Coarse Aggregate However, the cement quantity is less than that in IS Table 6: Mix Proportions method. After trial, if the required target strength is Cement Water FA CA (w/c) ratio 410 205 761.12 984 0.50 1 0.50 1.85 2.40 0.50 achieved & concrete is workable for a given application, it is acceptable. Volume of cement, Vc = 410/(3.15X1000)=0.130 m3. 3.6 Estimation of CA & FA Contents Table 5: Volume of CA Per Unit Volume of Concrete (SI Units) 4. COMPARISON OF IS METHOD & ACI METHOD FOR CONCRETE MIX DESIGN Table 7: Materials Required kg/m3) Met Cement Water FA (w/c) CA hod Ratio IS Let us assume that the fineness modulus of FA is 3. The ACI 426.67 192 703.42 1116.64 0.45 1 0.45 1.69 2.57 0.45 410 205 761.12 984 0.50 1 0.50 1.85 2.40 0.50 sand confirms to zone I as per IS code. From table 5, for 19 mm nominal max. size of aggregate, volume of dry rodded CA per unit volume of concrete is 0.60. 4.1 Observations So, mass of CA, Mca = (0.6 x dry rodded density of CA) = The cement content obtained by IS method is (0.6 X 1640) = 984 kg/m3 426.67 kg/m3; whereas, it is 410 kg/m3 as per ACI So, volume of CA, Vca = (Mca /Sp. gravity X 1000) method. = 984 / [2.72 x 1000] = 0.361 m3. With the same constituent materials, water per Volume of FA, Vfa = 1 – (Vc + Vw + Vca + Vea) m3, calculated by ACI method is 13 kg (or litres) Here, Vc = cement volume, Vw = volume of water, Vca= more than that obtained by IS method. volume of CA & Vea = volume of entrapped air (2%). Fine Aggregate quantity/m3 obtained by ACI Vfa = 1 - (0.130+ 0.205 + 0.361 + 0.02) = 0.284 method is 57.70 kg more than that obtained by IS Mass of FA, Mfa = (0.284 x 1000 x 2.68) = 761.12 kg. method. Yield of concrete = (410 + 205 + 984 + 761.12) = 2360.12 kg/m3. Coarse Aggregate quantity/m3 obtained by ACI method is 132.64 kg less than that obtained by IS method. Yield (i. e. density of concrete) is more in IS method of Mix Design. © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 2583 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 02 | Feb 2019 p-ISSN: 2395-0072 www.irjet.net 5. CONCLUSIONS ratio lowers & CA content becomes comparatively Looking at the proportions, it can be said that the more in IS method. At the same time, FA content Mix design by IS code is in line with that by ACI becomes less. method. From table 4 (ACI method), it can be depicted that the voids, thereby decreasing the strength of the compressive strength. However, IS code gives the concrete. max. limits for free (w/c) ratios depending upon the exposure conditions for plain concrete & RCC picking up a grade of M35. In doing so, certain Coarse Aggregates are more in IS method of mix modifications were done by manual judgment to design. fit to the requirements. Fine Aggregates are comparatively more in case of ACI method. should presumably lead to assumptions & modifications, using experience & more manual judgment, while carrying out Concrete workability, owing to the fact that the fine Mix Design may lead to somewhat deviating aggregates act as ball bearings & provide results. lubricating effect to the mix. As the Fine Aggregates have the tendency of filling number of trials in the laboratory for various due to enhanced particle packing. grades of concrete in order to simultaneously From table 5 (ACI method), it can be clearly seen satisfy strength & workability requirements. that if the nominal maximum size of CA & fineness REFRENCES modulus of FA are not varied then volume of dry rodded CA per unit volume of concrete is same for 1. Code of practice for plain and reinforced concrete any grade of concrete. In such a case, mass of the (fourth edition), IS 456:2000, Bureau of India CA is a function of dry rodded density of CA. If CAs Standard, New Delhi. are well graded with all size factions, there will be 2. Indian standard concrete mix proportioning - less voids. This will lead to higher dry rodded Guidelines (First revision) IS 10262:2009, Bureau density of CA. In ACI method, the mass of CA to be of India Standard, New Delhi, India. incorporated in concrete is independent of the One has to meticulously carry out Concrete Mix Design by both the methods & conduct a large the voids, ACI method should give more strength The results obtained just show a general trend in connection with both the methods. The different More quantity of Fine Aggregates, obtained by ACI method, This paper was an attempt of comparing the two methods of Concrete Mix Design by randomly work from durability point of view. This sounds contradictory theoretically, because of the possibility that more the CA, more would be (w/c) ratio to be used depends upon the required As the strength requirement increases, the (w/c) 3. Standard practice for selecting proportions for (w/c) ratio. normal, heavyweight, and mass concrete, ACI In IS method, as the (w/c) ratio decreases, the 211.1-91 (1991), ACI Committee 211, Farmington volume of CA increases. Vice versa is also true. Hills, MI, USA. Less the (w/c) ratio, more will be volume of CA which, in turn, leads to greater mass of CA. © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 2584